1.
Vivek Vanamane, Santhosh kumar B, Nataraj J. R./ International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp. 1550-1556 Characterization And Numerical Optimization Of Chromium Free Nickel Alloy Filler-Materials For Dissimilar Welding With SS304 Based On Induced Residual Stresses And Distortion Vivek Vanamane*, Santhosh kumar B**, Nataraj J. R.*** Department of Mechanical Engineering, R. V. College Of Engineering, Bangalore-59Abstract The aim of the work was to study and identify the compositional requirements to avoid theoptimize among eight different Cr free Ni based formation of deleterious phases such as eta phase,filler materials of chemical composition of wt% sigma phase and P-phase. Numerical simulation ofranging between 40-43.5Ni, 4-20Mo, 0-16Co, welding process using Finite Element Method10Cu, 22-25Fe, 0.5Al, 1Ti, 0.001C. The alloys (FEM) has been proved to be a powerful and usefuldeveloped were characterized for their method to predict the welding temperature field,metallurgical phases and mechanical properties residual stress field and deformation owing to thein both as-cast and solution treatment (at 1100 fact that, measurement of residual stress byºC) conditions using JMatPro V6 (materials experimental techniques has certain practicalsimulation software). The dissimilar welding of limitations. Experimental techniques may beSS 304 with these alloys is simulated using the destructive as the hole-drilling technique or evenbirth and death technique in ANSYS. Numerical when non-destructive techniques are used (e.g. X-Optimization was performed based on the ray diffraction technique), residual stress can beinduced stresses present in the weld joint which measured only at discrete locations near the weldare one of the main factors to cause failures in surface. The cost of performing these experimentsdissimilar weld joints. For welding simulation, would be a concerning factor, especially if largethe eight noded SOLID 70 elements were used for number of measurements are to be done. Lindgrenthermal stress analysis and SOLID 45 elements [4] gave a detailed account of the application of thewere used for structural analysis. The FEM Finite Element Method to predict the thermal,simulation results show the longitudinal residual material and mechanical effects of fusion weldingstresses along the weld line, tensile stresses from the 1970s to 2003. Chang and Teng et al [5]developed around 80 MPa occur at the middle of performed thermal elasto-plastic analyses using thethe weld. The maximum vertical deflection of finite element techniques to obtain the residual0.325 mm was observed for the alloy of stresses in the butt-welded joints. Goldak [6]composition 43.499Ni, 0.5Al, 14Co, 6Mo, 10Cu, introduced a 3D model for heat source generation.23Fe, 2Mn, 1Ti, 0.001C. On the other hand the Though, 3D heat source modeling provided accurateminimum vertical deflection of 0.2 mm and results but it requires lots of computation time.residual stress of 50MPa was observed in alloy of In the recent years, numerical optimization ofcomposition 39.999Ni, 0.5Al, 20Mo, 10Cu, 22Fe, various welding filler materials has been performed.6.5Mn, 1Ti, 0.001C. H. Naffakh [7] has performed dissimilar welding of AISI 310 austenitic stainless steel to nickel-basedKeywords: Alloy development, birth and death alloy Inconel 657, but no one has yet performed thetechnique, Finite Element Method, residual stress, numerical optimization of chromium free nickelWelding Simulation. alloy filler materials based on the induced residual stress in welding. This investigation performs1. Introduction thermal elasto-plastic analysis using finite element New chromium free Nickel based welding techniques to evaluate the residual stresses infiller materials for welding stainless steel were dissimilar welding. In this work about eight versionsimulated using JMatPro V6-materials simulation of chromium free Ni alloy filler materials ofsoftware). During TIG welding of stainless steel, chemical composition varying from 40-43.5%Ni, 4-carcinogenic Hexavalent Chromium Cr +6 fumes are 20%Mo, 0-16%Co, 10%Cu, 22-25%Fe, 0.5%Al,generated from the weld pool which can cause the 1%Ti, 0.001%C are optimised by determining thewelders respiratory problems including lung cancer. induced residual stresses using numerical simulation.OSHA in its new guidelines has reduced the A 2D surface heat flow model was implemented andPermission Exposure limit to 5μ/mm3 as explained the longitudinal and transverse stress distributionin the Welding Journals by Susan R. Fiore[1-2]. In was determined for all the alloys. Based on the2008, J. M. Vitek [3] demonstrated about how results of the analysis, the most suitable alloy forcomputational thermodynamics could be used to production of filler material for stainless steel welding is determined. 1550 | P a g e
2.
Vivek Vanamane, Santhosh kumar B, Nataraj J. R./ International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.2. Alloy Composition Table 1 shows the chemical composition ofthe various Nickel alloy filler materials consideredfor simulations. Cobalt, Iron, Molybdenum,Titanium, and Aluminum are all solid-solutionhardeners in Nickel. Cobalt having good solubilityof other alloying elements was varied from 0-16wt%. Cobalt wt% was balanced with Molybdenumwt%. Cobalt provides the dispersion ofstrengthening intermetallic particles. Higher Cobaltcontent imparts better wear resistance but lessdesirable polishability and machinability [1]. Thebeneficial influence of C in reducing sigma phase isdue to the fact that higher C leads to more carbideformation. The production of Ni based alloy for fig 2: JMatPro predicted Cooling Curve for Alloy 1Swelding electrodes has been increasing each yearowing to its good weldability, resistance to ductiledip cracking [8], hot cracking susceptibility, lesscarbon diffusion and high strength [9].3. JMatPro Results The various compositions were given inJMatPro software to determine the phases present atvarying temperatures. The phases present at 600°Care given in fig 1. fig 3: JMatPro predicted phase diagram of alloy type-1S 4. Experimental Results The cooling curves and microstructure of Alloy 1S was obtained experimentally and compared with JMatPro results. fig 2 predicts the cooling curve for the alloy type 1S, solidification begins at temperature 1270°C and ends at 1200 °C. JMatPro predicts existence of only liquid phase at the temperature above 1270°C as shown in fig 3. γ- solid solution phase exists between 1270-1200°C. Formation of MC type carbides phase is predicted at 1150°C. As the temperature falls below 990°C potentially undesirable phases including µ (mu) and eta η (eta) phase is predicted to form. γ’ (Gamma prime) precipitate phase is predicted to solidify below 750°C. In fig 4 DSC spectrum confirms thefig 1: % of phases of different alloys at 600°C prediction of JMAT Pro and fig 5 confirms the presence of alloying element in the XRD analysis. 1551 | P a g e
3.
Vivek Vanamane, Santhosh kumar B, Nataraj J. R./ International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp. 1550-1556Table: 1 Chemical composition of different version of Ni based alloys. Alloy Ni % Fe % Mo % Co % Cu % Mn % Ti % Al % C% 1S 39.999 22 20 Nil 10 6.5 1 0.5 0.001 2H 43.499 25 20 Nil 10 Nil 1 0.5 0.001 3N 43.499 25 10 10 10 0 1 0.5 0.001 4S 43.499 23 10 10 10 2 1 0.5 0.001 5N 43.499 23 6 14 10 2 1 0.5 0.001 6N 43.499 23 8 12 10 2 1 0.5 0.001 7S 43.499 23 12 8 10 2 1 0.5 0.001 8N 43.499 23 14 6 10 2 1 0.5 0.001 5. Thermo-Mechanical Analysis In this section, a sequential thermo-elastic plastic three-dimensional finite element computational procedure is developed to calculate temperature field, residual stresses and distortions. The procedure begins with a nonlinear transient thermal analysis and the temperature histories are applied as thermal loads in a nonlinear transient structural analysis to obtain the residual stresses and distortions. 6. Specimen and Material Propertiesfig 4: DSC cooling curve of Alloy type 1S fig. 7 shows two plate sections that are joined by a single-pass butt-weld. The length, width and thickness of the plate are assumed to be 140, 300 and 5 mm, respectively [10].fig 5: The XRD analysis of the 1S alloy confirms thepresence of Ni, Mo, Mn, Cu, Fe alloying elements. fig. 7 Shows two plate sections that are joined by a single-pass butt-weld Both thermal and mechanical material properties of 304 Stainless Steel were considered to be temperature-dependent and are given in Table 2. The thermal and mechanical properties of the 8 alloysa)As cast b) Solution Treated were obtained using JMAT Pro (Materials simulationfig 6: SEM Microstructures of Alloy software) and are given in the figures 8-11. Patches of lamellae, are clearly resolved athigher magnifications. In fig 6 Light, globularparticles are M6C; gray particles are MC carbide.Structures consist of nickel-rich γ solid-solutionmatrix containing a few light-etching carbide particlesand dispersed γ. JMatPro also indicates the presenceof M6C phase and MC carbide as shown in fig 1 for1S alloy. 1552 | P a g e
4.
Vivek Vanamane, Santhosh kumar B, Nataraj J. R./ International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.fig 8: Variation of Young’s Modulus of all alloys with fig 10: Variation of Thermal Expansion Coefficient ofTemperature. all alloys with Temperature.fig 9: Variation of Density of all alloys with fig 11: Variation of Thermal Conductivity of all alloysTemperature. with Temperature.Table 2. Thermal and mechanical material properties of SS304. Thermal ThermalTemperature expansion Density Specific heat Youngs Modulus conductivity(°C) Coefficient (kg/m3) (J/kg) (GPa) (W/m°C) (*10-6/°C)25 14.3489 16.76606 7749.77 462 206.21187100 14.3489 17.68191 7724.83 481.6 201.92657200 14.69002 18.90059 7690.46 517.8 195.4473300 15.03217 20.11912 7654.84 558.4 187.84373400 15.37537 21.34275 7618 608.6 179.11943500 15.71961 22.56949 7579.98 676.6 169.38741600 16.0649 23.78245 7540.8 784.4 158.8054700 16.41122 24.97985 7500.51 714.6 147.55249800 16.75859 26.17949 7459.14 672.4 135.82023900 17.10699 27.38602 7416.72 665.6 123.809361000 17.45644 28.59459 7373.29 671.6 111.728671100 17.80693 29.80303 7328.89 683.8 99.79361230 18.26413 31.37344 7269.79 746.6 84.86641350 18.29934 31.55186 7269.79 859.03 84.86697. 3D FE ModelThe three-dimensional finite element model used inthis simulation is shown in fig 12. The model has1148 elements and 2438 nodes after meshing. 1553 | P a g e
5.
Vivek Vanamane, Santhosh kumar B, Nataraj J. R./ International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp. 1550-1556 was defined relative to a coordinate system that was moving with the heat source is expressed as: Q’= (2) Where c is the arc radius, the total net heat input was calculated as: Q = UI (3) Where is the arc efficiency which is considered as 85%. This study simulates weld thermal cycle for SS 304 steel as shown in fig 13.fig 12: The finite element mesh for the single-pass The heating cycle takes 28 load stepsbutt-weld. increment with a time step of 1s and the modified Newton Raphson method was used in each time step The finite element meshes used for both for the heat balance iteration. Max temperature ofthermal and structural analyses are the same, except 1300° C is achieved during welding.for the element type. For thermal analysis, solid 70,an eight-node, first order brick element withtemperature degree of freedom at each node is used.For structural analysis, solid 45, an eight-node, firstorder brick element with three translational degreesof freedom. The constraints are provided as shownin fig 6 in order to allow free distortion of the plateduring welding [11].8. Thermal AnalysisThe transient temperature during welding isdetermined by the three-dimensional nonlinear heattransfer equation: fig 13: Simulated weld Thermal cycle for SS304 steel 9. Results and discussion(1) 9.1 Longitudinal residual stresses Where ρ is density, C is specific heat, k is Longitudinal stresses are the stresses actingthermal conductivity, Q is the rate of internal heat parallel to the weld bead and are denoted by y. fig.generation, T is temperature, t is time, and X, Y and 14 illustrates the distributions of the residual stressZ are coordinates in the reference system. y along the X-direction (at Y= 70 mm) for all the 8Convection heat transfer with a heat transfer alloys. High tensile stresses arise in regions near thecoefficient of 15 W/m2°C is applied to all free weld due to a resistance contraction of the materialsurfaces [12]. Radiation heat transfer is ignored. as cooling commences [12]. The stress distributionTable 3 shows the welding parameters chosen for is compressive in nature in the base metal region.this analysis. The minimum tensile residual stress of 51MPa is obtained for 1S alloy and a maximum tensile stressTable 3: Shows the welding parameters chosen for of 80MPa is obtained for 3N alloy.this analysis [13] Sl 9.2 Transverse residual stresses Parameter Value No Transverse residual stresses are the stresses 1 Welding Method TIG acting perpendicular to the weld bead and are 2 Current (I) 110 A denoted by x. fig. 15 represents the distributions of 3 Voltage (V) 20 V the residual stress x along the Y –direction for all 4 Welding Speed (v) 5 mm/s the alloys. As seen in the figure, the stress distributions are tensile in the middle of the weld The heat sources are applied along the weld and compressive at the ends [12]. The minimumpath for practical welds. A Gaussian power tensile residual stress of 50MPa is obtained for 1Sdistribution with an arc radius of 2.82 mm was alloy and a maximum tensile stress of 83MPa isassumed for the heat flux. The power distribution obtained for 5N alloy. 1554 | P a g e
6.
Vivek Vanamane, Santhosh kumar B, Nataraj J. R./ International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.9.3 Vertical Deflection recent years, the development of Cr free filler fig 16 shows the vertical deflection (in z materials have been on the rise due to noxiousnessdirection) along the length of the plates. As this of Cr+6 fumes generated during welding. 8 Ni basedfigure reveal, the maximum deflection is around alloys with varying composition of Cu, Co, Mn0.325mm which is sufficiently less. Due to property were developed and characterized for theirmismatch, a sharp variation in the deflection at the metallurgical phases and mechanical properties inweld is seen. Alloy 1S has a minimum deflection of both as-cast and solution treatment (at 1100 ºC)0.25mm at the weld. conditions using JMatPro V6. The use of JMatPro greatly reduces the cost and time required for the simulation and calculation. This can calculate wide range of materials properties for alloys and is particularly aimed at multi-components alloys used in industrial practice. Numerical Simulation using Finite Element Method reduces the time and cost of performing experimental analysis, especially if large number of measurements are to be done. The important results and conclusions extracted from this study are listed below. The experimental cooling curve of 1S alloy shows the solidification temperature as 1270C, JMatPro predicts existence of only liquid phase at temperature above 1270°C.fig 14: Longitudinal residual stress distribution The phases present at various temperatures asalong the X-direction. obtained from DSC spectrum matches with the prediction of JMatPro for 1S alloy. Numerical simulation of dissimilar welding of SS304 and the 8 alloys were performed using birth and death technique in ANSYS. The variation of residual stresses and distortion were determined. A minimum longitudinal tensile residual stress of 51MPa was obtained for 1S alloy and a maximum tensile stress of 80MPa was obtained for 3N alloy. The minimum transverse tensile residual stress of 50MPa was obtained for 1S alloy and a maximum tensile stress of 83MPa was obtainedfig 15: Transverse residual stress distribution along for 5N alloy. the Alloy 1S has a minimum deflection of 0.25mmY-direction. at the weld. From the results of Welding Simulation, 1S alloy was found to give less residual stresses and distortion than other alloys. Hence it can be concluded that 1S alloy with composition 39.999Ni, 0.5Al, 20Mo, 10Cu, 22Fe, 6.5Mn, 1Ti, 0.001C is more suitable compared to other alloys for dissimilar welding with SS304. Experimental Investigations can be performed on the weld samples in order to determine the strength and other properties of the weld in the future. References [1] ASM HandBook - Vol 02 - Properties andfig 16: Vertical Deflection along the width of the Selection Nonferrous Alloys and Special-plate. Purpose Materials(ASM International,1990)10. Conclusion [2] Susan r. Fiore, “Reducing Exposure to The above study involves the development Hexavalent Chromium in Welding Fumes”and optimization of 8 Cr free Ni based fillermaterials for dissimilar welding of SS304. In the 1555 | P a g e
7.
Vivek Vanamane, Santhosh kumar B, Nataraj J. R./ International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp. 1550-1556 Welding Journal, Edison Welding Institute, Engineering conference, KFUPM, Columbus, Ohi, August 2006. Dhahran, vol.5, De-2002, 297-312.[3] J. M. Vitek, D. W. Gandy2, “alloy [9] Changheui Jang, Jounghoon Lee, Jong development of nickel-based superalloy Sung Kim, Tae Eun Jin, “Mechanical weld filler metals using Computational property variation within Inconel 82/182 Thermodynamics”, 1 Oak Ridge National dissimilar metal weld between low alloy Laboratory, North Carolina 28262. steel and 316 stainless steel” International[4] L.-E. Lindgren, Numerical modelling of Journal of Pressure Vessels and Piping 85 welding, Computer Methods in Applied (2008) 635–646. Mechanics and Engineering 195 (48–49) [10] M. Seyyedian Choobi, M. Haghpanahi and (2006) 6710–6736. M. Sedighi. “Investigation of the Effect of[5] Chang, P.H., Teng, T.L., 2004. Numerical Clamping on Residual Stresses and and experimental investigations on the Distortions in Butt-Welded Plates”, IIW residual stresses of the butt-welded joints. International Congress on Welding & Comp. Mater. Sci. 29, 511–522. Joining, Tehran, Iran , 17( 5), pp. 387-[6] Goldak K, Chakaravarti A, Bibby M. A 394(2010). new finite element model for welding heat [11] Liam Gannon , Yi Liu , Neil Pegg , sources. Metallurgical Transactions Malcolm Smith, “Effect of welding 1984;15B:299–305. sequence on residual stress and distortion[7] H. Naffakha, M. Shamaniana, F. in flat-bar stiffened plates”, Marine Ashrafizadeha, Dissimilar welding of AISI Structures 23 (2010) 385–404. 310 austenitic stainless steel to nickel- [12] Tso-Liang Teng, Peng-Hsiang Chang, based alloy Inconel 657, Journal of Wen-Cheng Tseng. “Effect of welding Materials Processing Technology Volume sequences on residual stresses”, Computers 209, Issue 7, 1 April 2009, Pages 3628– and Structures 81 (2003) 273–286. 3639. [13] V. T. Bhanu Kiran, M. Krishna, Praveen[8] Gasem M Fallatah, Anwar K Sheik, M. and Niranjan Pattar. “Numerical Zafarullah khan, John K Boah, “Reliability Simulation of Multilayer Hard facing on of dissimilar metal welds subjected to Low Carbon Steel”, International Journal sulfide stress cracking”, The 6th Saudi of Engineering and Technology, Vol.3, No.1, February 2011, ISSN: 1793-8236. 1556 | P a g e
Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.
Be the first to comment